- Home
- Documents
*ON THE THEORY OF DIFFUSION-VISCOUS FLOW OF POLYCRYSTALLINE ... diffusion viscous flow of...*

prev

next

out of 12

View

7Download

1

Embed Size (px)

SOVIET PHYSICS JETP VOLUME 17, NUMBER 4 OCTOBER, 1963

ON THE THEORY OF DIFFUSION-VISCOUS FLOW OF POLYCRYSTALLINE BODIES

I. M. LIFSHITZ

Physic'o-technical Institute, Academy of Sciences, Ukrainian S.S.R.

Submitted to JETP editor November 20, 1962

J. Exptl. Theoret. Phys. (U.S.S.R.) 44, 1349-1367 (April, 1963)

The mechanism is analyzed and a quantitative theory is developed for the high-temperature diffusion viscous flow of polycrystalline bodies at low stresses. The role of slip along grain boundaries during their motion and diffusion deformation is explained. The viscosity coef- ficient tensor, which depends on the structural anisotropy of the substance (grain shapes and sizes) and on the magnitude of resistance to slip along grain boundaries, is derived. In addi- tion to the exact value of this tensor, simple interpolation formulas are given which permit investigation of the general flow equations. By way of example the kinetics of the filling-up of a spherical pore under pressure is considered. A study was made of the effects accom- panying the process of diffusion-viscous flow: the appearance of nonuniform stress fluctua- tions in a single grain (stresses of the second kind), variation of the macroscopic elastic moduli during flow, etc. The limits of applicability of the theory are discussed.

1. MECHANISM OF DIFFUSION-VISCOUS FLOW. STATEMENT OF THE PROBLEM

IT is known that, apart from the plastic flow of crystals, which is a threshold effect and occurs under sufficiently high loads, there is also a dif- fusion-viscous flow in solids at arbitrarily low stresses. The latter process is due to the dif- fusion of vacancies and is important only at high temperatures when this diffusion is sufficiently in- tensive. Strictly speaking, this process is domi- nant only at low stresses when all the other mech- anisms of a threshold nature (in particular the formation and motion of dislocations) are inactive.

The basic idea of the mechanism of diffusion- viscous flow was first put forward in the work of Nabarro [ 1] and Herring; [ 2] the latter work gives calculations and estimates for some typical cases of such flow. However, neither Nabarro nor Her- ring allowed for some important factors. Conse- quently there were many obscurities in their pic- ture of the process as a whole and in the conditions for its appearance, their estimates were not always valid. In the present work this mechanism is ana- lyzed from a somewhat different point of view and a derivation is given of a complete system of equa- tions describing the process of diffusion-viscous flow in the general case. At the same time the concomitant phenomena, typical of the mechanism of diffusion-viscous flow, become clear.

The first assumption in the mechanism of dif- fusion-viscous flow is that the surfaces bounding

structural units in a real crystalline body (separate grains in a polycrystal or separate blocks in a coarse-mosaic single crystal) are virtual sources and sinks for vacancies. In a perfect crystalline lattice a vacancy cannot be generated or annihilated by itself but a sufficiently defective surface repre- sents, as it were, an "amorphous" layer which is capable of reversible rearrangement when some vacancies reach it: it becomes as it were "com- pressed'' to its initial density and vacancies disap- pear. 1l

On the basis of this assumption the mechanism of flow is as follows: in a body subjected to a macroscopically uniform but anisotropic stress Uik• various normal stresses Uiknink (n is the vector normal to the surface) act on various por- tions of crystallite surfaces. Consequently near these surfaces the extent of saturation with vacan- cies varies: the chemical potential 1-1. of a vacancy at the surface (which is a virtual source of vacan- cies) will, by virtue of the equilibrium between the annihilation and generation of vacancies, be equal to

11- flo = kT In (c/c0) (1)

( c 0 is the equilibrium concentration of vacancies at p = 0; 1-'o is the chemical potential for the con- centration c0; w0 is the volume per unit vacancy);

1lAn analysis of the conditions under which a block boun- dary can be considered as a surface with virtual sources is given in Appendix 1.

909

910 I. M. LIFSHITZ

hence the value of the vacancy excess ll.c = c - co is determined by the relationship

(2)

The resultant concentration gradients within a grain give rise to diffusion currents of vacancies (or equiva- lent currents of atoms in the opposite direction). These currents produce a change of the grain shape without a change of its volume. The characteris- tic feature of this process is the absence of macro- scopic diffusion currents in the body as a whole and the presence only of complex microscopically nonuniform currents within each grain.

Deformation of the whole crystalline body con- sisting of a very large number of grains is a self- consistent process in the sense that discontinuities are not produced at the grain boundaries and the diffusion-viscous deformation of a particular grain depends on the deformations of the grains which surround it. The analysis given below shows that this necessarily produces stress fluctuations within each grain (stresses of the second kind) in spite of a macroscopically uniform stress state of the whole sample.

The self-consistent change in the shape of the grains is the result of the directional motion of their centers of gravity which produces macro- scopic changes in the shape of the body (flow). This displacement of the centers of gravity of the grains in diffusion-viscous flow is similar to the displacement of molecules in the process of the viscous flow of liquids, and is necessarily accom- panied by slip along grain boundaries.

If we introduce an average value of the stress tensor Pik = a ik in a small macroscopic element of volume containing a large number of grains, and also an average value of the velocities of displace- ment of particles in this element Vi = vi, then a macroscopic description of the process of flow is equivalent to the establishment of a relationship between the tensor Pik and the rate-of-deforma- tion tensor Vik = 1/ 2 ( &V/&xk + &Vk/&xd. In the general case of quasi-steady-state flow such a relationship should have the form

Vu = 0, (3)

where the viscosity tensor O!iklm is governed by the sizes and shapes of the grains, i.e., by the "structural anisotropy" of the polycrystal.

The equation of continuity Vii = 0 characterizes the aforementioned constancy of the grain volume and the absence of discontinuities. In the simplest case of structural isotropy O!iklm reduces to a scalar TJ and Eq. (3) becomes

- p = p 11 /3. (3a)

According to Eq. (2) the variation of the vacancy concentration oc on the grain surface is governed by the non-spherical (shear) part Pik = Pik + pc5ik of the stress tensor: oc = c0w0p' /kT. Therefore, the rate of deformation related to the diffusion currents h = D0&c/axi should be of the order of magnitude of

V;k ~D0a2c/3x;axk ~Dobc!L2 ~ p'Doe0wofL2kT

( L is the grain size). This gives an estimate of the expected magnitude of the viscosity tensor

O!iklm:

U;ktm ~ 1J ~ kTL2/Dw 0, D = Doeo

(Do is the vacancy diffusion coefficient and D is the atomic self-diffusion coefficient). We shall see, however, that this estimate is valid only in the case of free slip along grain boundaries.

The macroscopic coordinate dependence of the tensors Pik and Vik is determined by the equili- brium equation

(4)

which, together with Eq. (3), forms a complete sys- tem for the determinationofthe four quantities vi and p0:

apo a avt ax. + (fX Uikfm ax- = 0,

' k m div V = 0. (4a)

Thus our problem reduces to the derivation of Eq. (3) and the determination of aiklm in terms of the structural anisotropy of the polycrystal and the properties of the grain boundaries.

2. SELF-CONSISTENT DISPLACEMENT AND DEFORMATION OF GRAINS. ALIGNMENT OF STRESSES. ROLE OF SLIP ALONG GRAIN BOUNDARIES.

We shall consider a macroscopically uniform portion of the polycrystal (large compared with the grain dimensions) with given constant values of the average quantities Pik and Vik (Vii = 0). We shall select a microscopic element of volume (small compared with the grain dimensions) and follow its motion. The mass-current density, or in other words the average velocity v of this ele- ment, consists of a part va, related to the motion of the grain as a whole, and a part related to the vacancy-diffusion current j = - D0\7c; since the current of atoms is equal to the current of vacan- cies in the opposite direction, then 2>

2'Hereafter we shall assume that the diffu&ion coeffi- cient is isotropic.

THEORY OF DIFFUSION-VISCOUS FLOW OF POLYCRYSTALLINE BODIES 911

V=v"+D0 'Vc. (5)

From the continuity condition it follows that at the boundary of two grains denoted by a and {3 the normal components of the velocity Vn should be equal. According to Eq. (5) this gives the expres- sion

ac I ac I {l " Doarz a. -Doan ll = Vn-Vn, (6)

which represents the conditions for self-consistent motion of the grains and diffusion currents.

Since the concentration of vacancies is very small, only a negligibly small deformation ( ~ c0) can take place during the time necessary to estab- lish a quasi-steady-state diffusion current, and con- sequently during the whole process the distribution of vacancies is given by ~c == 0 (according to Eq. (5) this means div v == 0).